In the past decade, light-emitting diodes (LEDs) based on wideband gap semiconductor have attracted considerable attention due to its potential optoelectronic applications in illumination, mobile appliances, automotive and displays . Among the available wide band gap semiconductors, zinc oxide, with a large direct band gap of 3.37eV, is a promising candidate because of characteristic features such as a large exciton binding energy of 60meV, and the realization of band gap engineering to create barrier layers and quantum wells with little lattice mismatch. ZnO crystallizes in the wurtzite structure, the same as GaN, but, in contrast, large ZnO single crystal can be fabricated . Furthermore, ZnO is inexpensive, chemically stable, easy to prepare and etch, and nontoxic, which also make the fabrication of ZnO-based optical devices an attractive prospect. The commercial success of GaN-based optoelectronic and electronic devices trig the interest in ZnO-based devices [2-4].
Recently, the fabrication of
Figure1a shows the schematic structure of a typical ZnO homostructural p–i–n junction prepared by Tsukaza et al . The I-V curve of the device displayed the good rectification with a threshold voltage of about 7V (Figure1b). The electroluminescence (EL) spectrum from the p–i–n junction (blue) and photoluminescence (PL) spectrum of a p-type ZnO film at 300K were shown in Figure1c, which indicated that ZnO was a potential material for making short-wavelength optoelectronic devices, such as LEDs for display, solid-state illumination and photodetector.
White-light electroluminescence from n-ZnO)/p-GaN heterojunction LED was reported . The spectrum range from 400 to 700nm is caused by the carrier recombination at the interface between n-ZnO and p-GaN, as shown in Figure2, which makes ZnO as a strong candidates for solid-state light.
Currently, ZnO-based LEDs are leaping from lab to factory. A dozen or so companies are developing ultraviolet and white LEDs for market. The coloured ZnO-based LEDs have been produced by Start-up company MOXtronics, which shows its full-colour potential. Although the efficiency of these LEDs is not high, improvements are rapid and the emitters have the potential to outperform their GaN rivals. Figure3 shows some EL images of ZnO-based LEDs.
In this paper, based on the introduction of the band-gap engineering and doping in ZnO, we discuss the ZnO-based LEDs, comprehensively. We first discuss the band-gap engineering in ZnO, which is a very important technique to design ZnO-based LEDs. We then present the p- and n-types doping in ZnO. High quality n-type and/or p-type ZnO are necessary to prepare ZnO-based LEDs. Finally, we review the ZnO-based LEDs. In this part, we discuss homojunction ZnO LEDs and heterojunctions LEDs using
2. Band gap engineering in ZnO
Band gap engineering is the process of controlling or altering the band gap of a material by controlling the composition of certain semiconductor alloys. It is well known that tailoring of the energy band gap in semiconductors by band-gap engineering is important to create barrier layers and quantum wells with matching material properties, such as lattice constants, electron affinity for heterostructure device fabrication [2, 3].
Band-gap engineering in ZnO can be achieved by alloying with MgO, CdO or BeO. The energy band gap Eg(x) of ternary semiconductor AxZn1-xO (A = Mg, Cd or Be) can be calculated by the following equation:
Both MgO and CdO have the rock-salt structure, which is not the same as the ZnO wurtzite structure. When Mg and Cd contents in ZnO are high, phase separation may be detected, while BeO and ZnO share the same wurtzite structure and phase separation is not observed in BeZnO [2, 8]. Ryu et al studied the band gap of BeZnO and did not observed any phase separation when Be content was varied over the range from 0 to 100mol%. Figure4 shows the
Ohtomo et al investigated the band gap of MgxZn1-xO films grown on sapphire by PLD, where
Makino et al investigated the structure and optical properties of CdxZn1-xO films grown on sapphire (0001) and ScAlMgO4 substrates by PLD . The band gap of CdxZn1-xO films was estimated by Eg(y) = 3.29 − 4.40y + 5.93y2. The band gap narrowing to 2.99eV was achieved by incorporating Cd2+ with Cd concentration of 7%. Both lattice parameters a and c increase with the increasing Cd content in ZnO, which was agreement with the larger atomic size of Cd compared with Zn. CdxZn1-xO films were also prepared on c-plane sapphires by metal-organic vapor-phase epitaxy. The fundamental band gap was narrowed up to 300meV for a maximum Cd concentration of ~5%, introducing a lattice mismatch of only 0.5% with respect to binary ZnO. Lai et al prepared the CdxZn1-xO alloy by conventional solid-state reaction over the composition range and found that CdO effectively decreased the electronic bandgap both in the bulk and near the surface ZnO .
Using MgZnO as barrier layers, Chauveau et al prepared the nonpolar a-plane (Zn,Mg)O/ZnO quantum wells (QWs) grown by molecular beam epitaxy on r plane sapphire and a plane ZnO substrates . They observed the excitonic transitions were strongly blue-shifted due to the anisotropic strain state in heteroepitaxial QW and the reduction of structural defects and the improvement of surface morphology were correlated with a strong enhancement of the photoluminescence properties. Su et al investigated the optical properties of ZnO/ZnMgO single quantum well (SQW) prepared by plasma-assisted molecular beam epitaxy . The photoluminescence peak of the SQW shifted from 3.31 to 3.37eV as the well layer thickness was decreased from 6 to 2nm (Figure5). ZnO/MgZnO superlattices were also fabricated by laser molecular-beam epitaxy and the excitonic stimulated emission up to 373K was observed in the superlattices. The emission energy could be tuned between 3.2 and 3.4eV, depending on the well thickness and/or the Mg content in the barrier layers.
3. Doping in ZnO
ZnO has a strong potential for various short-wavelength optoelectronic device applications. To realize these applications, the reliable techniques for fabricating high quality n-type and p-type ZnO need to be established. Undoped ZnO exhibits n-type conduction due to the intrinsic defects, such as the Zinc interstitial (Zni) and oxygen vacancy (VO). It is easy to obtain the high quality n-type ZnO material by doping group-III elements. However, it is a major challenge to dope ZnO to produce p-type semiconductor due to self-compensation from native donor defects and/or hydrogen incorporation. To achieve p-type ZnO, various elements (N, P, As, Sb and Li) have been tried experimentally as p-type dopants with various techniques, such as pulse laser deposition, magnetron sputtering, chemical vapor deposition (CVD), molecular-beam epitaxy, hybrid beam deposition (HBD), metal organic chemical vapor deposition (MOCVD) and thermal oxidation of Zn3N2 [2, 3].
3.1. n-type ZnO
Kim et al reported the high electron concentration and mobility in AZO films grown on sapphire by magnetron sputtering . AZO films exhibited the electron concentrations and mobilities were of the order of 1018cm3 and less than 8cm2/Vs, respectively, however, when annealed at 9000C, the films showed remarkably improved carrier concentrations and mobilities, e.g., about 1020 cm3 and 45 – 65 cm2/Vs, respectively. Other researchers also reported the improved electrical properties in Al-doped zinc oxide by thermal treatment .
Bhosle et al investigated the electrical properties of transparent Ga-doped ZnO films prepared by PLD . Temperature dependent resistivity measurements for the films showed a metal-semiconductor transition, which was rationalized by localization of degenerate electrons. The lowest value of resistivity 1.4×10−4 Ωcm was found at 5% Ga. Yamada et al reported the low resistivity Ga-doped ZnO films prepared on glass by ion plating with direct current arc discharge . The ZnO:Ga film with a thickness of 98nm, exhibited a resistivity of 2.4×10−4 Ω cm, a carrier concentration of 1.1×1021cm−3 and a Hall mobility of 23.5cm2/Vs. Liang et al reported the Ga-doped ZnO films prepared on glass by magnetron sputtering and found that a carrier concentration exhibited only a slight change with the thickness variations .
Wang et al studied the properties of In-doped ZnO crystal by the hydrothermal technique . The indium-doped ZnO crystals have a resistivity lower than 0.015Ωcm with a free carrier concentration (mostly due to indium donors) of 1.09×1019/cm3 at room temperature. Quang et al reported the In-doped ZnO films grown by hydrothermal . The films had a mobility of 4.18-20.9cm2/Vs and a concentration of 6.7×1018 - 3.2×1019/cm3. The In-doped ZnO films with a carrier concentration of 3.22×1020/cm3 were grown by sol–gel method .
VII elements such as F and Cl are also used as n-type dopants in ZnO, which substituted oxygen ions. Cao et al reported F-doped ZnO grown by PLD with a minimum resistivity of 4.83×10-4 Ωcm, with a carrier concentration of 5.43×1020cm-3 and a mobility of 23.8cm2/ Vs . Chikoidze et al grew Cl-doped ZnO films by MOCVD with a resistivity of 3.6×10-3 Ω cm .
3.2. p-type ZnO
To realize ZnO-based LEDs, the most important issue is the fabrication of high quality p-type ZnO. However, undoped ZnO exhibits n-type conduction and the reliable p-type doping of the materials remains a major challenge because of the self-compensation from native donor defects (Vo and Zni) and/or hydrogen incorporation. Considerable efforts have been made to obtain p-type ZnO by doping different elements (N, P, As, Sb, Li, Na and K) with various techniques [2, 3]. Here, we present the typical results of p-type ZnO materials.
Among all potential p-type dopants for ZnO, N is considered the most promising dopant due to similar ionic radius compared with oxygen. It substitutes O sites in ZnO structure, resulting in the shallow acceptors. N2, NO, N2O, NH3 and Zn3N2 are acted as N sources depended on growth techniques [2, 3]. Liu et al reported p-type ZnO:N films grown on c-sapphire by plasma-assisted molecular beam epitaxy . The anomalous Raman mode at 275cm-1 was confirmed to be related to substitution of N for O site (NO) in ZnO. The films exhibited a hole concentration of 2.21×1016cm-3 and a mobility of 1.33cm2/Vs. Zeng et al investigated p-type ZnO films prepared on a-plane (11–20) sapphire by MOCVD . The optimized result was achieved at the temperature of 400°C with a resistivity of 1.72Ωcm, a Hall mobility of 1.59cm2/Vs, and a hole concentration of 2.29×1018cm−3. Wang et al prepared p-type ZnO films by oxidation of Zn3N2 films grown by direct current magnetron sputtering . For oxidation temperature between 350 and 5000C, p-type ZnO:N films were achieved, with a hole concentration of 5.78×1017cm-3 at 5000C. Kumar et al reported on the growth of p-type N,Ga-codoped ZnO films prepared by sputtering ZnO:Ga2O3 target in N2O ambient . The film deposited on sapphire at 5500C exhibited p-type conduction with a hole concentration of 3.9×1017 cm−3.
Beside N, other group V elements (P, As and Sb) are also used to be acceptor dopants to obtain p-type ZnO. However, first-principle calculations show that XO (PO, AsO and SbO) are deep acceptors and have high acceptor-ionization energies, owing to their large ionic radii as compared to O, which make it impossible for XO to dop ZnO efficiently p-type . We could not contribute the p-type behavious in X doped ZnO to XO, simply. Recently, for the large-size-mismatched impurities in ZnO, Limpijumnong et al proposed XZn−2VZn acceptor model . In the model, X substitute Zn sites, forming a donor, then it induces two Zn vacancy acceptors as a complex form XZn−2VZn. The ionization energy of AsZn - 2VZn complex was calculated to be 0.15eV (0.16eV for SbZn − 2VZn ).
Xiu et al reported p-type P-doped ZnO films grown by MBE using a GaP effusion cell as a phosphorus dopant source . PL spectra clearly indicated the existence of competitions between
Ryu et al investigated the electrical properties of As-doped ZnO films on O–ZnO substrates by hybrid beam deposition . The electrical behavior of ZnO:As films changed from intrinsic
Guo et al reported p-type ZnO:Sb films grown by PLD . The films showed a resistivity of 4.2 – 60Ωcm, a Hall mobility of 0.5 – 7.7cm2/V s, and a hole concentration of 1.9–2.2×1017cm−3. In the (HR) TEM images of p-type ZnO:Sb, they observed a high density of threading dislocations originating from the film/substrate interface and a large number of partial dislocation loops associated with small stacking faults. Xiu et al fabricated p-type ZnO:Sb films grown on n-Si (100) by MBE . The film had a concentration of 1.7×1018 cm−3, and a high mobility of 20.0cm2/Vs and a low resistivity of 0.2Ωcm. The acceptor energy level of the Sb dopant was about 0.2eV above the valence band, which was agreement with the ionization energy of SbZn − 2VZn (0.16eV).
Some researchers prepared p-type ZnO using Group I elements (Li, Na and K) as acceptor dopants. Yi et al fabricated p-type ZnO:Li films grown on quartz substrate by PLD with a hole concentration of 5.4×1018cm-3 . p-type ZnO:Na films were fabricated on Si substrates by PLD . The hole concentration ranged from 1.5×1018 to 1.1×1019 cm−3. Wu et al grew K-doped p-type ZnO films on (0001) Al2O3 substrates by radio frequency magnetron sputtering .
4. ZnO-based LEDs
4.1. Heterojunction LEDs
4.1.1. n-ZnO heterojunction LEDs
ZnO has attracted considerable attention because of its promising applications in UV LEDs and laser diodes. The fabrication of high-quality p-type ZnO remains great challenge. Many researchers reported on the heterojunction LEDs with n-type ZnO grown on p-type materials of Si, GaN and conducting oxides, as summarized in Table1.
Chang et al reported the MBE n-ZnO/MOCVD p-GaN heterojunction light-emitting diode . They grew 1-μm-thick undoped GaN buffer layer on Al2O3 and a 500-nm-thick Mg-doped p-GaN layer by MOCVD, and grew 300-nm-thick n-ZnO by MBE on p-GaN layer. They observed a broad yellowish green emission peaked at around 570nm. The EL emission was attributed to the electron injection from n-ZnO to p-GaN. Hwang et al fabricated an n-ZnO:Ga/p-GaN:Mg heterostructure on Al2O3 substrate . Undoped ZnO (buffer layer) and n-ZnO films doped with about 1% Ga were grown at 75W radio frequency (RF) power in 100% O2 atmosphere, at 8000C and 7000C, respectively. I-V characteristics exhibited the typical rectifying behavior and the EL emissions from the n-ZnO:Ga/p-GaN:Mg heterostructure at room temperature show peaks at 430nm, 440nm and 480nm along with a broad band of yellow light.
Lee et al investigated the origin of emission of the annealed n-ZnO/p-GaN heterostructure LED . They fabricated n-ZnO/p-GaN heterojunction LED on Al2O3 substrates by MOCVD (GaN layer) and RF sputtering (ZnO layer). After fabrication, ZnO films were annealed in a thermal furnace in air and nitrogen ambient at 800°C for 30–120min. For the LED annealed in N2, room-temperature EL in the blue region with peak wavelength 400nm was observed, and for the LED annealed in N2, a broad band from 400 to 700nm was detected in the EL emission spectrum, as shown in Figure6. Alivov et al reported the n-ZnO/p-AlGaN heterojunction light-emitting diodes on 6H-SiC substrates .
Chichibu et al fabricated p-CuGaS2/n-ZnO:Al heterojunction LEDs by metal-organic vapor phase epitaxy (p-CuGaS2) and helicon-wave-excited-plasma (HWEP) sputtering method (n-ZnO:Al) . The EL spectra exhibited emission peaks and bands between 1.6 and 2.5eV. Ohta et al reported on p-SrCu2O2/n-ZnO heterojunction LEDs . The I-V curve of the device exhibited nonlinear characteristics where the turn-on voltage was approximately 1.5V. An UV emission band centered at 382nm was observed at room temperature when a forward bias voltage greater than 3V was applied to the device, as shown in Figure7.
Ye et al reported the distinct visible electroluminescence at room temperature from
To improve the emission of n-ZnO-based heterojunction LEDs, dounble and triple heterojunction LEDs were fabricated. Osinsky et al reported MgZnO/ZnO/AlGaN/GaN triple heterostructures light-emitting diodes . I-V curves of the device showed a rectifying characteristics with a turn-on voltage of ~3.2 V. Strong optical emission was observed at ~390nm. Mares et al prepared a hybrid n-MgZnO/CdZnO/p-GaN LEDs with a Cd0.12Zn0.88O quantum-well . Under forward bias, visible electroluminescence was observed at room temperature in the EL spectrum of the device. The EL red shifted from 3.32 to 3.15eV as the forward current was increased from 20 to 40mA. Zhang et al investigated the effects of the crystalline and thickness of AlN layer on the electroluminescent performance of n-ZnO/AlN/p-GaN . They found that the better crystalline quality of AlN barrier layer may facilitate the improvement of EL performance of the device. For the thinner AlN layer, it was not enough to cover the whole surface of GaN, while in the thicker AlN layer, many of electrons were captured and nonradiatively recombined via the deep donors, indicating that AlN barrier layer played an important role on the performance of the device. In their experiments, AlN layer at the growth temperature of 7000C with an optimized thickness of around 10nm improved EL performance of the devices.
4.1.2. Heterojunction LEDs with ZnO nanomaterials
The optical devices using ZnO nanomterials have attracted considerable attention due to their promising optical properties, such as enriched radiative recombination of carriers. Various ZnO nanomaterials have been grown by different methods. Based on the growth of n-type ZnO nanomaterials, some researcher reported the heterojunction LEDs with ZnO nanomaterials, as summarized in Table2. Here, we only present the typical results on heterojunction LEDs with ZnO nanomaterials.
Xu et al reported ordered ZnO nanowire array blue/near-UV LEDs . The devices were fabricated by a conjunction of low temperature wet chemical methods and electron beam lithography. ZnO nanowire arrays were grown on Mg-doped p-type GaN films.
Zhang et al fabricated high-brightness blue-light-emitting diode using a ZnO-nanowire array grown on p-GaN thin film . The EL spectrum of the device showed broad emission peaks from UV (370nm) to blue. When the forward bias increased from 10 to 35V, the emission peak was significantly enhanced and the main emission peak shifted from 440 to 400nm when the forward bias was increased (Figure9), indicating that the modification of external voltage to the band profile in the depletion region. Lupan et al observed UV emission at 397nm with a low forward-voltage emission threshold of 4.4V and a high brightness above 5– 6V in ZnO-nanowire/p-GaN LEDs .
Alvi et al investigated the n-ZnO nanostructures (nanowalls, nanorods, nanoflowers and nanotubes)/p-GaN white-light-emitting diodes, systematically . In their experiments, ZnO nanostructures were grown on p-GaN substrates using a low temperature aqueous chemical growth method (<1000C) forming p – n heterojunctions. The EL spectrum of ZnOnanowall LED exhibited three peaks centered at 420nm (violet emission), 450nm (violet– blue) and broad peak covering from 480 to 700nm (green, yellow, orange and red emissions). For ZnO nanoflowers LEDs, the emission peaks centered at 400nm (violet emission), 450nm (violet–blue) and a broad peak covering EL emissions from 480 to 700nm (green, yellow, orange and red emissions) were detected. ZnO nanorods and nanotubes LEDs showed the same EL spectra, and EL peaks centered at 400nm (violet emission), 450nm (violet–blue) and 540nm (green emission) were observed. For ZnO nanostructures (nanowalls, nanorods, nanoflowers and nanotubes)/p-GaN LEDs, the color rendering indices (CRI) were 95, 93, 87 and 88, and the correlated color temperatures were 6518, 5471, 4807 and 4801K, respectively.
Xi et al fabricated heterojunction NiO/ZnO LEDs using low temperature solution-based growth method . The devices exhibited room-temperature electroluminescence, and the steady increase of the UV-to-visible emission ratio was obtained for increased bias voltage, which was good agreement with some of the reported behavior of ZnO LEDs.
Klason et al reported the EL spectra obtained from ZnO nanodots/p-Si heterojunction LEDs . The asymmetric EL emission peaked at around 600nm was observed and the emission from the devices having buffer layer were a bit blue shifted when compared to samples without the buffer layer. The buffer layer increased both the stability and efficiency of the devices.
Bano et al reported the ZnO-organic hybrid white LEDs grown on flexible plastic using low temperature aqueous chemical method . Figure10 shows the structure of ZnO-organic hybrid white LEDs, schematically. I-V curve of the device exhibited the typical rectifying behaviors. The EL spectrum displayed a broad emission band covering the whole visible region and hence provided white light. The white light emission was the superposition of a violet line (448nm), blue line (469nm) from the PFO combined with green emissions (503 and 541nm), and a red emission (620nm) due to deep level defect emissions in ZnO nanorods (Figure11). The color rendering index and correlated color temperature of the white LEDs were calculated to be 68 and 5800K, respectively (Figure12).
4.1.3. p-ZnO heterojunction LEDs
Currently, the fabrication of p-type ZnO materials has made remarkable progress and some researchers attempted to prepare p-type ZnO based hereojunction LEDs by various methods, as summarized in Table3.
Mandalapu et al reported ultraviolet emission from Sb-doped
Li et al reported on the blue electroluminescence from ZnO based heterojunction LEDs with CdZnO active layers .
Nakahara et al fabricated heterostructure LEDs by growing N-doped p-tye MgxZn1-xO layer by MBE on Zn face ZnO crystal using NO and NH3 as N source . The structures of the LEDs were shown in Figures16(a) and (b). The I-V curves of the LEDs exhibited a rectifying property [Figure16(c)]. LEDs A and B (NO as N source) had a turn-on voltage of approximately 3V, LEDs C and D (NH3 as N source) showed a turn-on voltage of 10V. In the EL spectra of LEDs A and B, a sharp EL peak at the near band edge (λ = 380 – 400nm) was seen, indicating an effective blocking of electrons by the wide band gap Mg0.1Zn0.9O:N layers and efficient exciton recombination in the
The EL peak energies of the LEDs were slightly lower than the PL peak energy of ZnO, which were due to the self-absorption of the ZnO emission in the thick ZnO substrate and the heating effect during the operation [Figure17(a)]. The outpower of the LEDs ranged from 0.1 to 70μW at the maximum attainable operation current (typically 30–40mA)[Figure17(b)]. Interestingly, when LED was coated with a 0.1-mm-thick epoxy resin containing 5wt % (BaEu)(MgMn)Al10O17 green phosphor, a part of ultraviolet NBE in the EL spectrum of the LED was converted into green, indicating that the UV emission may excite many existing phosphors developed for fluorescent tube and enable better color rendering [Figure17(c)].
Park et al reported on the growth and device properties of
4.1.4. Homojunction LEDs
Based on the fabrication of p-type ZnO materials, some researchers reported on ZnO-homojunction LEDs. Table4 is a survey of structure, method and emission peak of ZnO-homojunction LEDs.
Tsukaza et al fabricated ZnO p-i-n homojunction LEDs by laser MBE using N as acceptor dopant . The structure of the device was shown in Figure1(a). To realize an automatically flat interface, the homojunction structure was grown in layer-by layer. The I-V curve of the LED exhibited a rectifying behavior with a threshold voltage of 7V [Figure1(b)]. The threshold voltage was higher than the bandgap of ZnO (3.3eV), which was mainly attributed to the high resistivity of the p-type ZnO layer. The EL spectrum of the homojunction LED showed luminescence from violet to green regions with multi-reflection interference fringes. Compared PL spectrum of p-type ZnO and EL spectrum obtained from the LED, the higher energy side peak around 430nm in the EL spectrum matches well with the PL spectrum [Figure1(c)].
Chu et al reported on homojunction UV LEDs based on
Similarly, Kong et al fabricated Sb-doped
Wei et al prepared ZnO homojunction LEDs on
Sun et al reported on the ultraviolet electroluminescence from ZnO homojunction with
Ryu et al reported on ZnO-based UV LEDs fabricated by the hybrid beam deposition . The LEDs employed a BeZnO/ZnO active layer between
Figure20 shows the EL spectra of the LEDs at room temperature. The peaks centered 388nm (bound exciton — BE) and 550nm (green band — GB) were the dominant features at low forward currents (≤20mA), which were attributed the impurity (donor or acceptor)-bound exciton emission and donor-acceptor pair recombination. As the current injection levels was above 20mA, the peak at 363nm becomes the prominent spectral feature and the peaks at 388 and 550nm have become saturated. The peak at 363nm could be assigned to band-to-band recombination, such as from localized-exciton peaks in the active layer of the QWs.
Lim et al fabricated UV LEDs based on ZnO p-n homojunction . A Ga-doped ZnO layer (1.5μm) were grown on a c-Al2O3 substrates at 900°C by sputtering a ZnO target mixed with 1 wt% Ga2O3. A p-type ZnO layer (0.4μm) was grown in situ on the n-type ZnO layer at 900°C by sputtering a ZnO target mixed with 1 wt% P2O5. A rapid thermal annealing process was performed to the LEDs for 5min at 800°C in a nitrogen atmosphere in order to activate the p-type ZnO layers. The I-V curve of the device showed clear rectification with a threshold voltage of 3.2V, which was good agreement with the ZnO bandgap energy (3.37eV). The EL spectra of the ZnO homojunction LED is shown in Figure21. A NBE emission at 380nm and broad deep-level emissions at approximately 640nm were observed. The EL spectra of the LED matched well with the PL spectrum of the p-type ZnO film, indicating that the recombination of electrons and holes occurred mostly in p-type ZnO layer.
Sun et al reported on UV emission from a ZnO rod homojunction LED . Vertically aligned ZnO rods (Diameters: 200–500nm; Length:3.5μm) were uniformly grown on fluorine-doped tin oxide (FTO) coated sapphire
Figure24 displays the EL spectra of ZnO rod homojunction LEDs at various injection currents. Strong UV emission was observed from both devices, corresponding to the NBE emission of ZnO. The UV light output intensities increased linearly as injection current was above a threshold current (Figure23 insets). In addition, device I shows a relatively weak and broad emission band in the visible range, indicating a low density of deep-level defects, and the broad emission consisted of one green emission(~510nm) and one nearinfrared peak (~800nm) became stronger for device II. Similarly, Yang et al fabricated ZnO nanorod p-n homojunction LEDs with As implantation . The EL spectrum of the device exhibited a strong UV band centered at ~380 nm and a weak broad red band peaking at ~630nm.
5. Conclusion and outlook
With a large direct band gap of 3.37eV and a large exciton binding energy of 60meV, ZnO has attracted much attention for its application in optoelectronics applications, such as LEDs, photodetector and laser diodes. In the paper, based on the introduction of the band-gap engineering and doping in ZnO, we presented a comprehensive review of ZnO-based LEDs. Band-gap engineering in ZnO can be achieved by alloying with MgO, CdO or BeO. Theoretically, the energy band gap of AxZn1-xO can be continuously modulated from 0.9eV (CdO) to 10.6eV (BeO) by changing the A concentration. As a n-type semiconductor, high quality n-type ZnO materials can be obtained by doping doping III elements (Al, Ga and In). Although the fabrication of p-type ZnO remain great challenges due to the self-compensation, p-type ZnO have been prepared by doping different elements (N, P, As, Sb, Li, Na and K) with various techniques. ZnO based heterojunction and homojunction LEDs have been achieved, which makes ZnO as a strong candidates for solid-state light. Although the efficiency of ZnO-based LEDs is not high, improvements are rapid and the emitters have the potential to outperform their GaN rivals.
ZnO-based LEDs show great promise for the future, however, there are some severe issues that are in need of further investigation to transition ZnO-based LEDs to commercial use from the current stage. One problem is that the usable, reproducible p-type ZnO are not easy to fabricate, although some researchers have been successful. Another is the achievement of high quality p-n junction based ZnO. The p-n junction with good threshold and breakdown voltages is necessary for the LEDs. In addition, diode-like behavior and light emission have been observed, however, the mechanism of the properties remain unclear.
The work was supported by the Fundamental Research Funds for the Central Universities (Contract No: 531107040334) and the Aid Program for exploring investigation (Contract No: 513280501).
Choi Y-S, Kang J-W, Hwang D-K , Park S-J. Recent advances in ZnO-based light-emitting diodes, IEEE Trans. Electr. Dev. 2010; 57,26-41.
Janotti A, Van de Walle CG. Fundamentals of zinc oxide as a semiconductor, Rep.Prog.Phys.2009; 72, 126501 (29pages).
Özgϋr Ü, Alivov C, Liu C, Teke A, Reshchikov A, Doğan S, Avrutin V, Cho S-J, MorkoçH. A comprehensive review of ZnO materials and devices, J.Appl.Phys.2005; 98, 041301(103pages).
Look D.C., Recent advances in ZnO materials and devices, Mater.Sci.and Eng. B 2001; 80,383-387.
Tsukazaki A, Ohtomo A,Onuma T,Ohtani M, Makino T, Sumiya M, Ohtani K, ChichibuSF, Segawa Y, Ohno H, Koinuma H, Kawasaki M. Repeated temperaturemodulation epitaxy for p-type doping and light-emitting diode based on ZnO.Nat.Mater.2005; 4,42-46.
Chen SC, Chen MJ, Huang YH, Sun WC, Li W C, Yang J R. Kuan H, Shiojiri M. White-light electroluminescence fromn-ZnO/p-GaNheterojunctionlight-emitting diodes at reverse breakdown bias. IEEE Trans. Electron Devices2011; 58,3970-3975.
Ryu YR, Lee TS, LubgubanJ A, CormanA B, WhiteH W, Leem J H, Han M S, Park YS, Youn C J, Kim WJ. Wide-band gap oxide alloy:BeZnO. Appl.Phys.Lett.88, 052103(3pages).
Han MS, Kima JH, Jeonga TS, Parka JM, Youn CJ, Leem JH, Ryu YR. Growth and optical properties of epitaxial BexZn1-xO alloy films. J.Cryst.Growth 2007; 303, 506–509.
Ohtomo A, Kawasaki M, Koida T, Masubuchi K, Koinuma H, Sakurai Y, Yoshida Y, Yasuda T, Segawa Y. MgxZn1-xO as a II–VI wide-gap semiconductor alloy. Appl.Phys.Lett.1998;72, 2466-2468 (3pages).
Takagi T, Tanaka H, Fujita S, Fujita S. Molecular beam epitaxy of high magnesium content single-phase wurtzite MgxZn1−xO alloys (x similar or equal to 0.5) and their applicationto solar-blind region photodetectors. Jpn. J.Appl. Phys.2003;42, L401–L403.
Tampo H, Shibata H,Maejima K, Yamada A, Matsubara K, Fons P, Niki S, Tainaka T, Chiba Y, Kanie H. Strong excitonic transition of Zn1−xMgxO alloy. Appl.Phys.Lett.91, 261907(3pages).
Wassner T A, Laumer B, Maier S, Laufer A, Meyer B K, Stutzmann M, EickhoffM. (2009), Optical properties and structural characteristics of ZnMgO grown byplasma assisted molecular beam epitaxy. J. Appl.Phys.2009; 105, 023505 (6pages).
Makino T, Segawa Y, Kawasaki M, Ohtomo A, Shiroki R, Tamura K, Yasuda T, Koinuma H. Band gap engineering based on MgxZn1-xO and CdyZn1-yO ternaryalloy films. Appl.Phys.Lett.2001; 78, 1237-1239.
Lai H H-C, Kuznetsov V, Egdell RG, Edwards PP. Electronic structure of ternary CdxZn1-xO (0≤x≤0.075) alloy. Appl.Phys.Lett.100, 072106 (4 pages).
Chauveau J-M,Teisseire M, Kim-Chauveau H, Morhain C, Deparis O, Vinter B. Anisotropic strain effects on the photoluminescence emission fromheteroepitaxial and homoepitaxial nonpolar (Zn,Mg)O/ZnO quantum wells. J.Appl.Phys.109,102420 (6pages).
Su SC, Lu Y M, Zhang Z Z, Shan C X, Yao B, Li B H, Shen D Z, Zhang J Y, Zhao D X, Fan XW. The optical properties of ZnO/ZnMgO single quantum well grown by P-MBE. Appl. Surf. Sci.2008; 254, 7303–7305.
Kim K-K, Niki S, Oh J-Y, Song J-O, Seong T-Y, Park S-J, Fujita SZ, Kim S-W. High electron concentration and mobility in Al-doped n-ZnOepilayer achieved via dopant activation using rapid-thermal annealing. J.Appl.Phys.97,066103 (6pages).
Kim Y M, Lee W J, Jung D-R, Kim J M, Nam SH, Kim H C, Park BW. Optical and electronic properties of post-annealed ZnO:Al thin films. Appl. Phys. Lett. 2010; 96, 171902 (3pages).
Bhosle V, Tiwari A, Narayan J. Electrical properties of transparent and conducting Ga doped ZnO. J. Appl. Phys.2006; 100, 033713 (6pages).
Yamada T, Miyake A, Kishimoto S, Makino H, Yamamoto N, Yamamoto T. Low resistivity Ga-doped ZnO thin films of less than 100 nm thicknessprepared by ion plating with direct current arc discharge. Appl. Phys. Lett. 2007;91,051915(3pages).
Liang S, Bi X F. Structure, conductivity, and transparency of Ga-doped ZnO thin filmsarising from thickness contributions. J.Appl.Phys.2008;104,113533 (5pages).
Wang B G, Callahan MJ, Xu CC, Bouthillette LO, Giles NC, Bliss DF. Hydrothermal growth and characterization of indium-doped-conducting ZnO crystal.J. Cryst. Growth.2007; 304, 73-79.
Quang LH, Kuan LS, Liang GGK. Structural and electrical properties of single crystal indium doped ZnO films synthesized by low temperature solution method. J.Cryst.Growth2010; 312, 437-442.
Chen KJ, Hung FY, Chang SJ, Hu ZS. Microstructures, optical and electrical properties of In-doped ZnO thin films prepared by sol–gel method. Appl. Surf. Sci.2009; 255, 6308-6312.
Cao L, Zhu LP, Jiang J, Zhao R, Ye ZZ, Zhao BH. Highly transparent and conducting fluorine-doped ZnO thin films prepared by pulsed laser deposition. Sol. Energ. Mat.Sol. C.2011; 95, 894-898.
Chikoidze E, Modreanu M, Sallet V, Gorochov O,Galtier P. (2008), Electrical properties of chlorine-doped ZnO thin films grown byMOCVD, Phys. Stat. Sol. (A)2008; 205, 1575–1579.
Liu W W, Yao B, Zhang ZZ, Li WF, Li BH, Shan CX, Zhang J Y, Shen D Z, Fan XW. Doping efficiency, optical and electrical properties of nitrogen-dopedZnOfilms. J. App. Phys.2011; 109,093518 (5pages).
Zeng YJ, Ye ZZ, Xu WZ, Liu B, Che Y, Zhu LP, Zhao BH. Study on the Hall-effect and photoluminescence of N-dopedp-type ZnO thin films. Mater.Lett.2007; 61, 41-44.
Wang C,Ji ZG, Xi JH, Du J, Ye Z Z. Fabrication and characteristics of the low-resistive p-type ZnO thin films byDC reactive magnetron sputtering. Mater. Lett.2006; 60, 912-914.
Kumar M, Kim T-H, Kim S-S, Lee B-T. Growth of epitaxial p-type ZnO thin films by codoping of Ga and N. Appl. Phys. Lett. 2006;89,112103(3pages).
Park CH, Zhang SB, Wei S-H. Origin of p-type doping difficulty in ZnO: The impurity perspective. Phys. Rev. B2002; 66, 073202 (3pages).
Limpijumnong S, Zhang S B, Wei S-H, Park CH. Doping by large-size-mismatched impurities: the microscopic origin of ArsenicorAntimony-doped p-type Zinc Oxide. Phys. Rev.Lett.2004; 92,15504 (4pages).
Xiu FX, Yang Z, Mandalapu L J, Liu J L. Donor and acceptor competitions in phosphorus-doped ZnO. Appl. Phys. Lett.2006; 88, 152116 (3pages).
Kim K K, Kim H-S, Hwang DK, Lim J-H, Park S-J. Realization of p-type ZnO thin films via phosphorus doping and thermalactivation of the dopant. Appl. Phys. Lett.2003;88, 152116 (3pages).
Pan X H, Jiang J, Zeng Y J, He H P, Zhu L P, Ye Z Z, Zhao B H, Pan X Q. Electrical and optical properties of phosphorus-doped p-type ZnO filmsgrown by metalorganic chemical vapor deposition. J.Appl.Phys.2008;103,023708(4pages).
Vaithianathan V, Lee B-T,Kim SS. Pulsed-laser-deposited p-type ZnO films with phosphorus doping. Appl. Phys. Lett.2005; 98, 043519 (3pages).
Ryu Y R, Lee T S, Leem J H, White H W, Fabrication of homostructuralZnOp–n junctions and ohmic contactsto arsenic-doped p-type ZnO. Appl. Phys. Lett.2003;83,4032-4034.
Vaithianathan V, Lee B-T, Kim S S. Preparation of As-doped p-type ZnO films using a Zn3As2 /ZnO targetwith pulsed laser deposition. Appl. Phys. Lett.2005;86,062101 (3pages).
Kang HS, Kim GH, Kim DL, Chang HW, Ahn BD, Lee SY. Investigation on the p-type foramtion mechanism of arsenic-dopedp-type ZnOthim films. Appl. Phys. Lett. 2006; 89, 181103(3pages).
Guo W, Allenic A, Chen YB, Pan XQ, Che Y, Hu Z D, Liu B. Microstructure and properties of epitaxial antimony-doped p-type ZnO filmsfabricated by pulsed laser deposition.Appl. Phys. Lett.2007; 90,242108 (3pages).
Xiu FX, Yang Z, Mandalapu L J, Zhao DT, Liu JL, Beyermann YP. High-mobilitySb-doped p-type ZnO by molecular-beam epitaxy. Appl. Phys. Lett.2005; 87,152101 (3pages).
Yi JB, Lim CC, Xing GZ, Fan HM, Van LH, Huang SL, Yang KS, Huang XL, Wang BY, Wu T, Wang L, Zhang HT, Gao XY, Liu T, Wee ATS, Feng Y.P, Ding J. (2010), Ferromagnetism in dilute magnetic semiconductors through defect engineering: Li-doped ZnO. Phys.Rev.Lett.2010;104,137201 (4pages).
Lin SS, He HP, Lu YF, Ye ZZ.Mechanism of Na-doped p-type ZnO films: Suppressing Na interstitials bycodoping with H and Na of appropriate concentrations. J.Appl.Phys.2009;106, 093508(5pages).
Wu J, Yang YT. Deposition of K-doped p type ZnO thin films on (0001) Al2O3substrates. Mater.Lett.2008; 62, 1899-1901.
Chang SP, Chuang RW,Chang SJ, Chiou YA,Lu CY. MBE n-ZnO/MOCVDp-GaNheterojunction light-emitting diode.Thin Solid Films 2009; 517, 5054-5056.
Wang SP, Shan CX, Zhu H, Li B H,Shen D Z, Liu XY, Tang Z K. Phosphor-converted light-emitting diode based on ZnO-based heterojunction. J. Lumin.2010;130, 2215-2217.
Zheng H, Mei ZX, Zeng Z Q, Liu Y Z, Guo LW, Jia JF, Xue Q K, Zhang Z, Du X L. Fabrication and characterization of high quality n-ZnO/p-GaNheterojunction lightemission diodes.Thin solid films2011; 520, 445- 447.
Mares J W, Falanga M,Thompson AV, Osinsky A,Xie J Q, Hertog B, Dabiran A, Chow PP, Karpov S, Schoenfeld W V. Hybrid CdZnO/GaN quantum-well light emitting diodes.J.Appl.Phys.2008; 104,093107 (5pages).
Osinsky A, Dong GW, Kauser MZ, Hertog B, Dabiran AM, Chow PP, Pearton SJ, Lopatiuk O, Chernyak L. MgZnO/AlGaNheterostructure light-emitting diodes. Appl.Phys.Lett.2004; 85,4272-4274.
Hwang S-H, Chung TH, Lee BT. Study on the interfacial layer in ZnO/GaNheterostructure light-emitting diode.Mater.Sci.Eng.B2009;157, 32-35.
Lee JY, Lee JH, Kim HS, Lee CH, Ahn H-S, Cho HK, Kim YY, Kong BH, Lee HS. A study on the origin of emission of the annealed n-ZnO/p-GaNheterostructure LED. Thin Solid Films2009;517, 5157-5160.
Han W S, Kim Y Y, Kong BH, Cho H K. Ultraviolet light emitting diode with n-ZnO:Ga/i-ZnO/p-GaN:Mgheterojunction. Thin solid films2009; 517, 5106-5109.
Zhang SG, Zhang XW, Yin ZG, Wang JX, Dong JJ, Wang ZG,Qu S, Cui B, Wowchak AM, Dabiran AM, Chow P P. Improvement ofelectroluminescent performance of n-ZnO/AlN/p-GaNlight-emitting diodes by optimizing the AlN barrier layer. J. Appl.Phys.2011; 109, 093708 (6pages).
Iwan S, Bambang S, Zhao JL., Tan ST, Fan HM, Sun L, Zhang S, Ryu HH, Sun XW. Green electroluminescence from an n-ZnO: Er/p-Si heterostructured light-emitting diode. Physica B, http://dx.doi.org/10.1016/j.physb.2012.03.072 .
Ohta H, Kawamura K-I, Orita M, Hirano M, Sarukura N, Hosono H. Current injection emission from a transparent p –n junction composedof p-SrCu2O2/n-ZnO. Appl.Phys.Lett.2000;77, 475-477.
Rogers DJ, Teherani F H, Yasan A, Minder K, Kung P, Razeghi M. Electroluminescence at 375 nm from a ZnO/GaN:Mg/c-Al2O3heterojunction light emitting diode. Appl.Phys.Lett.2006; 88,14198 (3pages).
Yu QX, XuB, Wu Q H, Liao Y, Wang GZ, Fang RC. Optical properties of ZnO/GaNheterostructure and its near-ultravioletlight-emitting diode. Appl. Phys. Lett.2003; 83, 4713-4715.
Ye J D,Gu S L ,Zhu S M, Liu W, Liu SM, Zhang R, Shi Y, Zheng Y D. Electroluminescent and transport mechanismsof n-ZnO/p-Siheterojunctions. Appl.Phys.Lett.2006; 88, 182112 (3pages).
Li XP, Zhang BL, Zhu HC, Dong X, Xia XC, Cui YG,Ma Y, Du GT. Study on theluminescence properties ofn-ZnO/p-Si hetero-junction diode grownby MOCVD.J. Phys. D: Appl. Phys. 2008; 41, 035101(5pages).
Alivov YI, Kalinina EV,Cherenkov AE, Look DC, Ataev BM, Omaev AK, Chukichev MV. Bagnall DM. Fabrication and characterization of n-ZnO/p-AlGaNheterojunctionlight-emitting diodes on 6H-SiC substrates. Appl. Phys.Lett.2003; 83, 4719-4721.
AlivovY I, Nostrand JEV, Look DC, Chukichev MV, Ataev BM. Observation of 430nm electroluminescence from ZnO/GaNheterojunctionlight-emitting diodes.Appl.Phys.Lett.2003; 83, 2943-2945.
Chichibu SF, Ohmori T, Shibata N, Koyama T, Onuma T. Fabrication of p-CuGaS2/n-ZnO: Alheterojunction light-emittingdiode grown by metalorganic vapor phase epitaxy andhelicon-wave-excited-plasma sputtering methods. J. Phys. Chem.Solids2005; 66, 1868-1871.
Xu S, Xu C, Liu Y, Hu YF, Yang RS, Yang Q, Ryou J-H, Kim HJ, Lochner Z, Choi S, Dupuis R, Wang ZL. Ordered nanowire array blue/near-UV light emitting diodes. Adv.Mater.2010;22, 4749-4753.
Bano N, Zaman S, Zainelabdin A, Hussain S, Hussain I, Nur O, Willander M. (2010), ZnO-organic hybrid white light emitting diodes grown on flexible plasticusing low temperature aqueouschemical method. J. Appl.Phys.2010;108, 043103 (5pages).
Guo Z, Zhang H, Zhao D X, Liu YC, Yao B, Li B H, Zhang Z Z, Shen D Z. The ultralow driven current ultraviolet-blue light-emitting diode basedon n-ZnO nanowires/i-polymer/p-GaNheterojunction. Appl. Phys. Lett.2010; 97, 173508 (3pages).
Alvi NH, Usman Ali SM, Hussain S, Nur O, Willander M. Fabrication and comparative optical characterization of n-ZnO nanostructures (nanowalls, nanorods, nanoflowers and nanotubes)/p-GaN white-light-emitting diodes. Scripta.Mater. 2011; 64, 697-700.
Willander M, Nur O, Zaman S, Zainelabdin Z, Banon, Hussain I. (2011), Zinc oxide nanorods/polymer hybridheterojunctions for white lightemitting diodes.J. Phys. D: Appl. Phys. 2011; 44 , 224017(6pages).
Zhang X M,Lu M-Y, Zhang Y, Chen L-J, Wang Z L. Fabrication of a high-brightness blue-light-emitting diode using a ZnO-nanowire array grown on p-GaN thin film. Adv.Mater.2009; 21, 2767-2770.
Chang C-Y, Tsao F-C, Pan C-J, Chi G-C, Wang H-T, Chen J-J, Ren F, Norton D P, Pearton S J, Chen K-H, Chen L-C. Electroluminescence from ZnO nanowire/polymer composite p-n junction. Appl. Phys. Lett.2006;88,173503(3pages)
Klason P, Rahman MM, Hu Q-H, Nur O, Turan R, Willander M. Fabrication and characterization of p-Si/n-ZnOheterostructured junctions. Microelectronics Journal2009; 40,706-710.
Lee S W, Cho H D, Panin G, Kang T W, Vertical ZnOnanorod/Si contact light-emitting diode. Appl. Phys. Lett.2011;98,093110(3pages)
ParkW I, YiG C.Electroluminescence in n-ZnOnanorod arraysvertically grown on p-GaN, Adv. Mater.2004;16, 87–90.
ParkS H, KimS H, HanS W. Growth of homoepitaxial ZnO film on ZnO nanorods and light emitting diode applications. Nanotech.2007;18, 055608 (6pages).
Lupan O, Pauporté T, Viana B. Low-voltage UV-electroluminescence from ZnO-nanowirearray/p-GaNlight-emitting diodes. Adv. Mater.2010; 22,3298–3302.
Zhang QB, Guoa HH, Feng ZF, Lin LL, Zhou JZ, Li ZH. n-ZnOnanorods/p-CuSCNheterojunction light-emitting diodes fabricated byelectrochemical method. Electrochim.Acta2010;55, 4889 – 4894.
Xi YY, Hsu YF, Djurišić AB, NgAMC, Chan WK, Tam HL, Cheah KW. NiO/ZnO light emitting diodes by solution-based growth. Appl.Phys.Lett.2008; 92,113505 (3pages).
Guo R, NishimuraJ, Matsumoto M, Higshihata M, Nakamura D, Okada T. Electroluminescence from ZnO nanowirebasedp-GaN/n-ZnOheterojunction light-emittingdiodes. Appl. Phys.B, Photophys. Laser Chem.2009;94, 33–38.
Mandalapu LJ,Yang Z, Chu S, Liu JL. Ultraviolet emission from Sb-doped p-type ZnO based heterojunctionlight-emitting diodes. Appl.Phys.Lett.2008; 92,122101 (3pages).
Li L, Yang Z, Kong JY, Liu JL. Blue electroluminescence from ZnO based heterojunction diodeswith CdZnO active layers. Appl.Phys.Lett.2009; 95, 232117 (3pages)
Nakahara K, Akasaka S, Yuji H, Tamura K, Fujii T, Nishimoto Y, Takamizu D, Sasaki A, Tanabe T, Takasu H, Amaike H, Onuma T, ChichibuS F, Sukazaki A,Ohtomo A, Kawasaki M. Nitrogen doped MgxZn1−xO/ZnO single heterostructure ultravioletlight-emitting diodes on ZnO substrates. Appl.Phys.Lett.2010; 97, 013501 (3pages).
Park T-Y, Choi Y-S, Kim S-M, Jung G-Y, Park S-J, Kwon B-J, Cho Y-H. Electroluminescence emission from light-emitting diode ofp-ZnO/(InGaN/GaN)multiquantum well/n-GaN. Appl.Phys.Lett.2011;98, 251111 (3pages)
Sun J C, Feng Q J, Bian JM, Yu DQ, Li MK, Li CR, Liang HW, Zhao JZ, Qiu H, Du GT. Ultraviolet electroluminescence from ZnO-based light-emitting diode with p-ZnO:N/n-GaN:Siheterojunction structure. J. Lumin.2011; 131, 825-828.
Hwang D-K, Kang S-H, Lim J-H, Yang E-J, Oh J-Y, Yang J-H, Park S-J. p-ZnO/n-GaNheterostructureZnO light-emitting diodes. Appl.Phys.Lett.2005; 86, 222101 (3pages).
Choi H-K, Park J-H, Jeong S-H, Lee B-T. Realization of As-doped p-type ZnO thinfilms using sputter deposition. Semicond. Sci. Technol. 2009;24,105003(4pages).
Kim YY, Han WS, Cho HK. Determination of electrical types in the P-doped ZnO thin films by the control of ambient gas flow. Appi.Surf.Sci.2010;256, 4438-4441.
Kim HS, Lugo F, Pearton S J, Norton D P, Wang Y-L, Ren F. Phosphorus doped ZnO light emitting diodes fabricated via pulsedlaser deposition. Appl. Phys. Lett.2008;92,112108(3pages).
Tay C B, Chua S J, Loh K P. Stable p-type doping of ZnO film in aqueous solution at low temperatures. J. Phys. Chem. C2010; 114, 9981–9987.
Wei ZP, Lu YM, Shen DZ, Zhang ZZ, Yao B, Li BH, Zhang JY, Zhao DX, Fan XW, Tang ZK. Room temperature p-n ZnO blue-violet light-emitting diodes. Appl.Phys.Lett.2007; 90, 042113 (3pages).
Chu S, Lim JH, Mandalapu LJ,Yang Z, Li L, Liu J L. (2008), Sb-doped p-ZnO/Ga-dopedn-ZnOhomojunction ultraviolet light emittingdiodes. Appl.Phys.Lett.2008; 92,152103 (3pages).
Kong JY, Chu S, Olmedo M, Li L,Yang Z, Liu J L. Dominant ultraviolet light emissions in packed ZnO columnarhomojunction diodes. Appl.Phys.Lett.2008; 93,132113 (3pages).
Liu W,Gu SL,Ye J D,Zhu SM, Liu S M, Zhou X, Zhang R,Shi Y, Zheng YD,Hang Y, Zhang CL. (2006), Blue-yellow ZnOhomostructural light-emitting diode realizedby metalorganic chemical vapor deposition technique. Appl.Phys.Lett.2006;88, 092101 (3pages).
Sun J C, Zhao J Z, Liang H W, Bian J M, Hu L Z, Zhang H Q, Liang X P., Liu W F, Du GT. Realization of ultraviolet electroluminescence from ZnOhomojunctionwithn-ZnO/p-ZnO:As/GaAs structure. Appl.Phys.Lett.2007; 90, 121128 (3pages).
Sun JC, Liang HW, Zhao JZ, Bian JM, Feng QJ, Hu LZ, Zhang HQ, Liang XP, Luo YM, Du GT. Ultraviolet electroluminescence from n-ZnO:Ga/p-ZnO:Nhomojunction device on sapphire substrate with p-type ZnO:N layer formed by annealing in N2O plasma ambient. Chem.Phys.Lett.2008; 460, 548-551.
Gu QL, Ling CC, Brauer G, Anwand W, Skorupa W, Hsu YF, Djurišić AB, Zhu CY,Fung S,Lu LW. Deep level defects in a nitrogen-implanted ZnO homogeneous p-n junction. Appl.Phys.Lett.2008; 92, 222109 (3pages).
Yang Y, Sun X. W, Tay B K, You G F, Tan S T,Teo KL. (2008), A p-n homojunctionZnOnanorod light-emitting diode formedby As ion implantation. Appl.Phys.Lett.2008;93,253107 (3pages).
Sun X W, Ling B, Zhao J L,Tan ST, Yang Y, Shen YQ, Dong Z L, Li CX. Ultraviolet emission from a ZnO rod homojunction light-emitting diode. Appl.Phys.Lett.2009; 95,133124 (3pages).
LimJ H, Kang C K, Kim K K, ParkI K, Hwang D K, Park S J. UV electroluminescence emission from ZnOlight-emittingdiodes grown by high-temperature radio frequency sputtering.Adv.Mater.2006; 18, 2720–2724.
Fang X, Li JH, Zhao D X, Shen DZ, Li B H, Wang X H. Phosphorus-doped p-type ZnOnanorods and ZnOnanorod p-n homojunction LED fabricated by hydrothermal method. J. Phys. Chem. C2009; 113, 21208–21212.
Ryu Y R, Lee T-S, Lubguban J A, White H W, Kim BJ, Park YS, Youn C J. (2006), Next generation of oxide photonic devices: ZnO-based ultraviolet lightemitting diodes. Appl.Phys.Lett. 2006; 88, 241108 (3pages).